The discovery of nanostructured carbon materials such as fullerenes (Kroto et al., 1985) and carbon nanotubes (Iijima, 1991) has led to a considerable interest in the development of various carbonaceous materials. In particular, porous carbonaceous materials have been attracting much attention because of their high surface area, large pore volume, chemical inertness, and high mechanical stability. Porous carbons show promise in the fields of hydrogen-storage, catalysis, separation, nanoreactors, electrochemistry, and biochemical engineering. Traditional synthesis methods, which involve carbonization of activated carbon (Marsh et al., 1971; Tamai et al., 1996; Hu et al., 2000), produce only disordered materials. To date, fabrication of highly ordered structure remains challenging. Research efforts to produce porous carbon materials with well-tailored pore systems have focused on the use of various inorganic template materials such as porous anodic aluminum oxide (AAO) films (Kyotani et al., 1995, 2006), zeolites (Kyotani et al., 1997; Ma et al., 2000; Nishihara et al., 2009), siliceous opals (Zakhidov et al., 1998; Yu et al., 2002), and mesoporous silicas (Ryoo et al., 1999; Lee et al., 1999; Kaneda et al., 2002; Kleitz et al., 2003; Xia et al., 2006) to template the carbon.
The use of zeolites, which have 3-dimensionaly connected framework structures constructed from corner-sharing TO4 tetrahedra, where T is any tetrahedrally-coordinated cation such as Si and Al, as templates for the synthesis of carbon deposits on the micropore walls has been successful. The resulting materials have ordered and uniform angstrom-sized pores. However, long-range ordered microporous carbon replicas require repetitive carbonization steps to completely fill the template pores.
Silica opals, also called colloidal crystals, which are made by the self-assembly of uniform submicrometre-sized silica spheres, have been used as templates for the synthesis of ordered macroporous carbons. The porosity and contact sites between the silica spheres provided walls and interconnected spherical pores, respectively, in the resulting carbons.
Similarly, synthesis of ordered mesoporous carbons has focused on the use of ordered mesoporous silicas with interconnected pore structures as templates. Ordered structures of mesoporous silicas are derived from the self-assembly of surfactants and silica precursors. The development of the M41S family (Kresge et al., 1992; Beck et al., 1992; Zhao et al., 1998) triggered the synthesis of a wide variety of mesoporous materials with diverse symmetries using various surfactants. As a result, various mesoporous carbon nanostructures with different pore systems have been synthesized using a variety of different mesoporous silica templates (Fig. 1). Pore size is controllable by selecting silica templates of different lengths and adjusting the silica wall thickness, though there is no report of tailoring only the silica wall thickness of the mesoporous silicas with constant pore diameter.
All the above inorganic-templating techniques require (1) preparation of inorganic templates, (2) impregnation of template pores with appropriate carbon precursors, (3) carbonization, and (4) subsequent selective removal of the templates using hydrofluoric acid or sodium hydroxide (Fig. 2). It is interesting to note that the pore system of carbons is inversely replicated from the silica templates, and thus, various mesostructured carbons with different pore systems have been synthesized using a variety of different mesoporous silica templates. Often, this time-consuming and costly process requires multiple infiltrations to complete the filling of the template pores. It is difficult to perform pore filling of the carbon precursors into the mesopores of silicas with low accessible pore systems.
Alternative methods, which eliminate the need for an inorganic template, have recently been developed to synthesize highly ordered mesoporous carbons, by directly assembly of organic templates with the carbon precursors (Tanaka et al., 2005, 2007, 2009; Meng et al., 2005; Zhang et al., 2005, 2006; Jin et al., 2009, 2010; Simanjuntak et al., 2009). This strategy uses an organic–organic interaction between a thermosetting resin and a thermally-decomposable copolymer to form a periodic ordered nanocomposite. The thermosetting
resin remains as the carbonaceous pore walls, while thermally-decomposable copolymer decomposes to form the mesopores (Fig. 2).
Simple techniques to control morphology and configuration of ordered mesoporous carbons are required for the development of practical applications. In this chapter, an advantageous organic-templating method for morphology control of ordered mesoporous carbons is introduced.
2. Self-assembly of organic–organic nanocomposites
In the inorganic-templating method, variable carbon precursors, e.g., sucrose, furfuryl alcohol, naphthalene, acetylene, polyacrylonitrile, and phenolic resin, can be utilized. On the other hand, in the organic-templating method, the main carbon precursors have been phenolic polymer resins prepared using phenolic resin monomer and formaldehyde (Fig. 3). The major reactions between phenolic resin monomer and formaldehyde include an addition reaction to form methylene and hydroxymethyl derivatives to form methylene and methylene ether bridged compounds. Interestingly, it has been pointed out that the polymerization mechanism and structure of resorcinol/formaldehyde are analogous to that described for the sol–gel processing of silica (Pekala 1989).
The commercially available Pluronic block copolymers, e.g., F127, P123, and F108, have been used as templates (Fig. 3). To fabricate mesostructure, it is important to adjust the chemistry of the template head groups that can fit the requirement of the carbon precursors. The molecular interaction between the template head group and framework precursor can be expected using conventional reaction schemes. Six different possible molecular reaction pathways which use the principle of surfactant liquid crystal templating have been identified: (S+Fˉ), (S–F+), (S+XˉF+), (SˉX+Fˉ), (SºFº), and (S–F), where S is the surfactant (cationic S+, anionic S–, neutral Sº), F is the soluble framework precursor (cationic F+, anionic Fˉ, neutral Fº), and X is the intermediated (cationic X+, anionic Xˉ) molecular species (Fig. 4). S–F indicates systems where the framework specie is covalently bonded to the template. The pathway applicable to a particular synthesis will be dictated by the reagents and synthesis conditions and can be influence the physical and chemical properties of the product. Hydrogen-bonding interaction between the copolymer template and the phenolic polymer resin is an efficient route to prepare mesoporous carbons (Fig. 5).
2.1. Synthesis of ordered mesoporous carbons using organic templates
In a typical synthesis, phenolic resin monomers were completely dissolved in a mixture composed of deionized water, ethanol and hydrochloric acid. Pluronic F127 was then added, and after it was completely dissolved, formaldehyde (37 wt.%) was added to the solution. The final molar composition of the solution was 4 phenolic resin monomers : 1 : 0.005–0.05 Pluronic F127 : 9 formaldehyde : 0.1 HCl : 20–100 ethanol : 40 water. The solutions were left at room temperature, during which they separated into two phases. The transparent upper phase was ethanol–water rich and the lower dark brown phase was polymer-rich. The upper clear phase was discarded; the lower dark brown phase was preheated at 100º C for 1 h in air. Subsequently, the resultant brown sample was carbonized under a nitrogen atmosphere at 200–800º C.
On the basis of the thermosetting resorcinol/formaldehyde resins, ordered mesoporous carbons, designated as COU, have been synthesized via the triblock copolymer F127-
templating route with the addition of triethyl orthoacetate as a co-carbon source. Fig. 6 shows X-ray diffraction (XRD) patterns of ordered mesoporous carbons COU-1. XRD pattern revealed a sharp reflection peak at a 2
The surfactant F127 must have decomposed below 400º C, because mesopores were already generated in the COU-1 carbonized at 400º C. The thermosetting RF polymer remained as the carbonaceous pore walls, while the Pluronic F127 decomposed to form the mesopores. The increase in the micropore volume and the BET surface area at 600º C must be due to the generation of gases from the decomposition of the RF polymer. The molar ratios of C/H were increased with increasing the carbonization temperature. The large increase in the C/H ratio at 800º C indicates that the decomposition of the RF polymer still continued at 600–800º C, although the micropore volume and the BET surface area showed no further increase above 600º C.
2.2. Synthesis of hierarchically ordered mesoporous carbons
Although the inorganic-templating method is quite attractive, one should keep it in mind that this technique requires both the use of an expensive template and its removal by a severe treatment, which hampers the practical use of the template technique. On the other hand, because the template can be water-soluble in the organic-templating technique, the process would be much simpler and could be performed at low cost. Furthermore, it is noted that the organic-templating approach is advantageous for controlling the morphology and configuration and one can be use the inorganic template, which have larger template structure than that of Pluronic triblock copolymer, for preparation of mesoporous carbons with hierarchical porous structures.
The use of AAO films, which have uniform straight channels with 10–250 nm diameters, as templates for the synthesis of carbon deposits on the channel walls has been successful (Kyotani et al., 1995, 2006). The resulting tubular carbon materials have tunable diameters, lengths, and wall thickness. Additionally, the uniformity of the carbon nanostructures had never been seen before in carbon nanotubes when compared with carbon nanostructures prepared by conventional arc-evaporation or catalytic chemical vapor deposition (CVD) techniques.
On the other hand, a method to fabricate mesostructured silica within columnar pores of the AAO membranes via the surfactant-templating method has been developed (Yamaguchi et al., 2004). When ordered mesoporous silica is synthesized in film morphology, the mesostructure tends to orient with a specific (
The procedure is quite simple and rapid; the films of triblock copolymer F127–templated phenolic polymer resin can be deposited at the columnar pore surface of the AAO membrane by simply immersing the membrane in the precursor solution. AAO membrane (average pore diameter = 200 nm, thickness = 60 μm, membrane diameter = 25 mm) was set in an ordinary membrane filtration apparatus, and the precursor solution described above was dropped onto it (Fig. 9). Moderate aspiration was applied so that the solution penetrated into the columnar alumina pores. The membrane including the precursor solution was dried in air. Carbonization was performed as described above. The AAO scaffold was completely removed by immersing the composite membrane in alkali solution.
Fig. 10 shows TEM images of mesostructured carbon nanofibers embedded within the pores of AAO membranes and released by dissolving the AAO membrane. A well-ordered structure can be obtained and the mean diameter of the mesopores in the carbon nanofibers is approximately 8 nm. The results of N2 adsorption/desorption analysis of the mesoporous carbon nanofibers attached to the AAO membrane revealed that the pore diameter is 7.6 nm, which is in good agreement with TEM observations.
Hydrothermal stability and alkaline resistance of the nanofibers were investigated by TEM observation before and after immersing in 5 M NaOH solution at 100º C for 24 h. For nanofibers carbonized at 400º C, the ordered mesostructure collapses completely after alkaline hydrothermal treatment, because the framework is still composed of an intermediate between a polymer and carbon. In contrast, for nanofibers carbonized at 600 and 800º C, the mesostructures show no difference before and after treatment. Thus,
nanofibers carbonized at high temperatures (above 600º C) show high hydrothermal stability and alkaline resistance. The longitudinal dimension and diameter of the nanofibers are about 60 μm and 200 nm, respectively, which are consistent with the pore dimension of the AAO membranes. The structural order seems to become distorted in the interior region. At the fiber–air interface, ordered layers with a short-range-order structure seem to be oriented along the interface in different directions, as indicated by the arrows.
2.3. Synthesis of ordered mesoporous carbon films and membranes
Development of well-ordered mesoporous carbon films will lead to new applications such as separation membranes and electronic devices. In the inorganic-templating method, the use of mesoporous silica thin films, rather than bulk powders, are unsuitable as a template because of the lack of pore accessibility in the silica films. Then, it is difficult to maintain the continuous film and film adhesion to the substrate may become poor.
In this section, a simple synthesis of mesoporous carbons in thin film and membrane (thick film) morphologies by means of organic–organic self-assembly using phenolic resin monomers and Pluronic F127 is introduced. Completely continuous films composed of ordered mesoporous carbon can be obtained by dip-coating or spin-coating.
Fig. 11 shows an FESEM image of a cross-section of ordered mesoporous carbon film. The color of the film turned black after carbonization at 400º C. A continuous and flat film about 600 nm thick was grown from the silicon substrate. The carbon films were tightly adhered to the substrate even after carbonization at 800º C. Increasing ethanol/water molar ratio and consequent decreasing concentration of the component decreases film thickness. In addition, film thickness can be controlled by adjusting the withdrawal rate during dip-coating.
When ordered mesoporous materials are synthesized in film morphology, the mesostructure tends to orient with a specific (
The molar ratio of phenolic resin monomers to F127 was changed from 115 to 800 by varying the concentration of the F127. The films prepared at phenolic resin monomers/F127 molar ratio of 200 and 160 are referred to as CKU-F69 and CKU-C12, respectively. GISAXS patterns were collected from CKU-F69 films carbonized at temperatures from 200 to 800º C (Fig. 12). Interpretation of the GISAXS patterns was aided by NANOCELL (Tate et al., 2006), a program which simulates quantitatively the positions of Bragg diffraction peaks based on the distorted-wave Born approximation (DWBA) to account for the effects of refraction and reflection at the film–substrate and film–air interfaces. The experimental results were fitted to a face-centered orthorhombic
Upon the initial assembly, it is conjectured that the mesostructure is described by the body-centered lattice, likely a (110) oriented
The ordered mesostructures were also preserved during this high temperature carbonization process. However, the interplanar distance,
The pores have an ellipsoidal shape due to anisotropic contraction upon drying and the carbonization process, in contrast to isotropic contraction for bulk powders without a support medium. Besides the uniformity of the pore size, the pore shape may be useful for limiting the sizes or orientations of guest molecules in separation, catalysis, and sensor applications. From TEM observations, it was found that many domains exist and are oriented parallel to the substrate with different rotational directions. Highly ordered patterns of cage-like pores support the conclusion that CKU-F69 products possess orthorhombic
Microporous and mesoporous inorganic membranes have been investigated mainly with respect to silica membrane prepared by the sol–gel method (Park et al., 2001; Nishiyama et al., 2003; Sakamoto et al., 2007). However, silicate materials dissolved in water and alkaline solutions, which decrease the possibility of practical use. On the other hand, carbon membranes have attracted increasing interest because of their advantages, such as high surface area, high hydrothermal stability, and chemical inertness. Ordered mesoporous carbon is a promising material in the field of membrane filtration technologies, such as nanofiltration and ultrafiltration.
Next, mesoporous carbon membranes were prepared on the porous α-alumina support. α-Alumina porous tubular supports (outer diameter: 10 mm, inner diameter: 7 mm, length: 35mm, average pore size: 100 nm, average porosity: 40%) were purchased from Noritake Co., Ltd., Japan. To prepare cylindrical porous α-alumina tubes with dead-end structure, a 20 mm section of the porous α-alumina tube was joined to a dense α-alumina tube (outside diameter: 10 mm, inner diameter: 7 mm, length: 250 mm) and an α-alumina disk (diameter: 12 mm, thickness: 2 mm) with a SiO2–BaO–CaO sealant and then calcined at 1100º C. Membranes were prepared by dip-coating the α-alumina porous tubular support in the coating solution.
A continuous and smooth layer about 5 μm thick was formed on the support surface. From the EDX analysis, the membrane had a carbon/alumina composite layer with a thickness of about 3.5 μm because a coating solution penetrated into the alumina pores. The ordered mesostructures were also preserved during this high temperature carbonization process, although the carbonization of the membrane shrunk the ordered structure, which corresponds to 5% contraction. Gas permeation measurements were carried out using N2 to confirm the compactness of the membranes. In the permeation test, a total pressure on the feed side was kept constant in the range of 75–180 kPa and the permeate side was kept constant at atmospheric pressure. The permeance of N2 through the alumina support increased with increasing the pressure drops, suggesting that the contribution of viscous flow cannot be negligible for the alumina support. In contrast, the permeances of N2 through the mesoporous carbon membranes were independent of the pressure drops across the membranes. The N2 gas permeance through the mesoporous carbon membranes is predominantly governed by the Knudsen diffusion (Uhlhorn et al., 1989). These results strongly indicate that there are no important pinholes and/or defects in the membranes.
The moisture and alkaline resistance is one of the most important factors in the filed of membrane separation (Park et al., 2001; Nishiyama et al., 2003). The membranes were placed under extremely severe hydrothermal conditions (90º C, in water) and in alkaline solution (at pH 12, for 1 week). The ordered mesostructure and gas permeation properties of the carbon membrane carbonized at 600º C were maintained.
2.4. Control of mesostructure; effect of ethanol/water ratio
Table 1 summarizes the results of the pore structure analysis. The
The pore size increases with increasing ethanol/water molar ratio. Control of pore size is one of the most important subjects in the study of mesoporous materials, and many methods for achieving control have been reported. The most common methods focus on the use of various swelling agents such as 1,3,5-trimethylbenzene (Beck et al., 1992), 1,3,5-triisopropylbenzene (Kimura et al., 1998), and decane (Blin et al., 2000). The strategy here is that a micellar array in which the core is composed of hydrophobic hydrocarbon chains participates in the solubilization of hydrophobic molecules. Incremental addition of the swelling agent results in an increasing pore size. This method has been shown to lead to pore expansion of up to 30%, usually accompanied by a loss of the long-range order of the mesostructure. In the organic-templating method for preparation of ordered mesoporous carbons, ethanol seems to play an important role in determining the characteristics of the porous structure. It is well known that the aqueous phase behavior of surfactants is influenced by the presence of short-chain alcohols (
interface to help stabilize liquid crystals and determine their surface curvatures. The method for controlling the mesostructure composed of silica using a ternary triblock copolymer–butanol–water system has been reported, as well as similar systems using pentanol and hexanol instead of butanol (Feng et al., 2000; Kleitz et al., 2004; Kim et al., 2005). The addition of these alcohols, which act as cosurfactants or swelling agents, results in not only increased pore size but also formation of a mesophase with a decreased curvature.
Fig. 13 shows that the mesophase may change with the micellar interfacial curvature, which varies with ethanol content. Ethanol swells the hydrophobic volume of the triblock copolymer micelles and interacts with both PPO and PEO segments because it is highly polar molecule. Thus, ethanol is located at the hydrophilic–hydrophobic interface (PEO/PPO) and stabilizes the interface, leading to the formation of micellar aggregates with decreased interfacial curvature.
As has been demonstrated in this chapter, the organic-templating approach is a very powerful method for the preparation of various types of ordered mesoporous carbons. The supramolecular templating technique opens an avenue for ordered mesoporous carbons and has advantages for controlling the morphology and configuration. The recent progress made in the development of organic-templating method was reviewed. Research efforts to produce ordered mesoporous carbons have focused on the use of phenolic polymer resins and thermally-decomposable Pluronic triblock copolymers. The choice of an appropriate set of thermosetting polymers and thermally-decomposable organic templates is the most important factor in controlling the mesophase topologies and morphology control of ordered mesostructured carbons. In powder preparation by simple precipitation process, the addition of ethanol expands both the pore size and
This work was supported by the Kinki Invention Center, the Murata Science Foundation (A91153), and the Japan Society for the Promotion of Science (JSPS) (KAKENHI #19860074 and #21760562). The GISAXS patterns were collected at the NSF funded facility for In-situ X-ray Scattering from Nanomaterials and Catalysts (MRI program award 0321118-CTS). The authors thank Dr. M. P. Tate and Associate Prof. H. W. Hillhouse (Purdue University) for the GISAXS measurements.
Kroto H. W. Heath J. R. O’Brien S. C. Curl R. F. Smalley R. E. 1985C-60-buckminsterfullerene, , 318 6042 162 163, 0028-0836
Iijima S. 1991Helical microtubules of graphitic carbon, , 354 6348 56 58, 0028-0836
Marsh H. Rand B. 1971The process of activation of carbons by gasification with CO2-II. The role of catalytic impurities, , 9 1 63 72, 0008-6223
Tamai H. Kakii T. Hirota Y. Kumamoto T. Yasuda H. 1996Synthesis of extremely large mesoporous activated carbon and its unique adsorption for giant molecules, , 8 2 454 462, 0897-4756
Hu Z. Srinivasan M. P. Ni Y. 2000Preparation of mesoporous high-surface-area activated carbon, , 12 1 62 65, 0935-9648
Kyotani T. Tsai L. F. Tomita A. 1995Formation of ultrafine carbon tubes by using an anodic aluminum-oxide film as a template, , 7 8 1427 1428, 0897-4756
Kyotani T. 2006Synthesis of various types of nano carbons using the template technique, , 79 9 1322 1337, 0009-2673
Kyotani T. Nagai T. Inoue S. Tomita A. 1997Formation of new type of porous carbon by carbonization in zeolite nanochannels, , 9 2 609 615, 0897-4756
Ma Z. Kyotani T. Tomita A. 2000Preparation of a high surface area microporous carbon having the structural regularity of Y zeolite, , 23 2365 2366, 1359-7345
Nishihara H. Yang Q. H. Hou P. X. Unno M. Yamauchi S. Saito R. Paredes J. I. Martinez-Alonso A. Tascon J. M. D. Sato Y. Terauchi M. Kyotani T. 2009A possible buckybowl-like structure of zeolite templated carbon, , 47 5 1220 1230, 0008-6223
Zakhidov A. A. Baughman R. H. Iqbal Z. Cui C. Khayrullin I. Dantas S. O. Marti J. Ralchenko V. G. 1998Carbon structures with three-dimensional periodicity at optical wavelengths, , 282 5390 897 901, 0036-8075
Yu J. S. Kang S. Yoon S. B. Chai G. 2002Fabrication of ordered uniform porous carbon networks and their application to a catalyst supporter, , 124 32 9382 9383, 0002-7863
Ryoo R. Joo S. H. Jun S. 1999Synthesis of highly ordered carbon molecular sieves via template-mediated structural transformation, , 103 37 7743 7746, 1089-5647
Lee J. Yoon S. Hyeon T. Oh S. M. Kim K. B. 1999Synthesis of a new mesoporous carbon and its application to electrochemical double-layer capacitors, , 21 2177 2178, 1359-7345
Kaneda M. Tsubakiyama T. Carlsson A. Sakamoto Y. Ohsuna T. Terasaki O. Joo S. H. Ryoo R. 2002Structural study of mesoporous MCM-48 and carbon networks synthesized in the spaces of MCM-48 by electron crystallography, , 106 6 1256 1266, 1520-6106
Kleitz F. Choi S. H. Ryoo R. 2003Cubic Ia3d large mesoporous silica: synthesis and replication to platinum nanowires, carbon nanorods and carbon nanotubes, , 17 2136 2137, 1359-7345
Xia Y. Yang Z. Mokaya R. 2006Simultaneous control of morphology and porosity in nanoporous carbon: Graphitic mesoporous carbon nanorods and nanotubules with tunable pore size, , 18 1 140 148, 0897-4756
Kresge C. T. Leonowicz M. E. Roth W. J. Vartuli J. C. Beck J. S. 1992Ordered mesoporous molecular-sieves synthesized by a liquid-crystal template mechanism, , 359 6397 710 712, 0028-0836
Beck J. S. Vartuli J. C. Roth W. J. Leonowicz M. E. Kresge C. T. Schmitt K. D. Chu C. T. W. Olson D. H. Sheppard E. W. Mc Cullen S. B. Higgins J. B. Schlenker J. L. 1992A new family of mesoporous molecular-sieves prepared with liquid-crystal templates, , 114 27 10834 10843, 0002-7863
Zhao D. Huo Q. Feng J. Chmelka B. F. Stucky G. D. 1998Nonionic triblock and star diblock copolymer and oligomeric surfactant syntheses of highly ordered, hydrothermally stable, mesoporous silica structures, , 120 24 6024 6036, 0002-7863
Tanaka S. Nishiyama N. Egashira Y. Ueyama K. 2005Synthesis of ordered mesoporous carbons with channel structure from an organic-organic nanocomposite, , 16 2125 2127, 1359-7345
Tanaka S. Katayama Y. Tate M. P. Hillhouse H. W. Miyake Y. 2007Fabrication of continuous mesoporous carbon films with face-centered orthorhombic symmetry through a soft templating pathway, , 17 34 3639 3645, 0959-9428
Tanaka S. Doi A. Nakatani N. Katayama Y. Miyake Y. 2009Synthesis of ordered mesoporous carbon films, powders, and fibers by direct triblock-copolymer-templating method using an ethanol/water system, , 47 11 2688 2698, 0008-6223
Jin J. Tanaka S. Egashira Y. Nishiyam N. 2010KOH activation of ordered mesoporous carbons prepared by a soft-templating method and their enhanced electrochemical properties, , 48 7 1985 1989, 0008-6223
Jin J. Nishiyama N. Egashira Y. Ueyama K. 2009Pore structure and pore size controls of ordered mesoporous carbons prepared from resorcinol/formaldehyde/ triblock polymers, , 118 1-3, 218 223, 1387-1811
Simanjuntak F. H. Jin J. Nishiyama N. Egashira Y. Ueyama K. 2009Ordered mesoporous carbon films prepared from 1,5-dihydroxynaphthalene/triblock copolymer composites, , 47 10 2531 2533, 0008-6223
Meng Y. Gu D. Zhang F. Q. Shi Y. F. Yang H. F. Li Z. Yu C. Tu B. Zhao D. 2005Ordered mesoporous polymers and homologous carbon frameworks: Amphiphilic surfactant templating and direct transformation, , 44 43 7053 7059, 1433-7851
Zhang F. Q. Meng Y. Gu D. Yan Y. Yu C. Z. Tu B. Zhao D. 2005A facile aqueous route to synthesize highly ordered mesoporous polymers and carbon frameworks with Ia3d bicontinuous cubic structure, , 127 39 13508 13509, 0002-7863
Zhang F. Q. Meng Y. Gu D. Yan Y. Chen Z. X. Tu B. Zhao D. 2006An aqueous cooperative assembly route to synthesize ordered mesoporous carbons with controlled structures and morphology, , 18 22 5279 5288, 0897-4756
Pekala R. W. 1989Organic aerogels from the polycondensation of resorcinol with formaldehyde, , 24 9 3221 3227, 0022-2461
Yamaguchi A. Uejo F. Yoda T. Uchida T. Tanamura Y. Yamashita T. Teramae N. 2004Self-assembly of a silica-surfactant nanocomposite in a porous alumina membrane, , 3 5 337 341, 1476-1122
Hillhouse H. W. Egmond J. W. Tsapatsis M. Hanson J. C. Larese J. Z. 2001The interpretation of X-ray diffraction data for the determination of channel orientation in mesoporous films, , 44-45, 639 643, 1387-1811
Tanaka S. Tate M. P. Nishiyama N. Ueyama K. Hillhouse H. W. 2006Structure of mesoporous silica thin films prepared by contacting PEO106-PPO70-PEO106 films with vaporized TEOS, , 18 23 5461 5466, 0897-4756
Tate M. P. Urade V. N. Kowalski J. D. Wei T. C. Hamilton B. D. Eggiman B. W. Hillhouse H. W. 2006Simulation and interpretation of 2D diffraction patterns from self-assembled nanostructured films at arbitrary angles of incidence: From grazing incidence (above the critical angle) to transmission perpendicular to the substrate, , 110 20 9882 9892, 1520-6106
Park D. H. Nishiyama N. Egashira Y. Ueyama K. 2001Enhancement of hydrothermal stability and hydrophobicity of a silica MCM-48 membrane by silylation, , 40 26 6105 6110, 0888-5885
Nishiyama N. Saputra H. Park D. H. Egashira Y. Ueyama K. 2003Zirconium-containing mesoporous silica Zr-MCM-48 for alkali resistant filtration membranes, , 218 1-2, 165 171, 0376-7388
Sakamoto Y. Nagata K. Yogo K. Yamada K. 2007Preparation and CO2 separation properties of amine-modified mesoporous silica membranes, , 101 1-2, 303 311, 1387-1811
Uhlhorn R. J. R. Keizer K. Burggraaf A. J. 1989Gas and surface-diffusion in modified gamma-alumina systems, , 46 23 225 241, 0376-7388
Kimura T. Sugahara Y. Kuroda K. 1998Synthesis of mesoporous aluminophosphates using surfactants with long alkyl chain lengths and triisopropylbenzene as a solubilizing agent, , 5 559 560, 1359-7345
Blin J. L. . Otjacques C. Herrier G. Su B. L. 2000Pore size engineering of mesoporous silicas using decane as expander, , 16 9 4229 4236, 0743-7463
Ekwall P. Mandell L. Fontell K. 1969The cetyltrimethylammonium bromide-hexanol-water system, , 29 4 639 646, 0021-9797
Feng P. Y. Bu X. H. Pine D. J. 2000Control of pore sizes in mesoporous silica templated by liquid crystals in block copolymer-cosurfactant-water systems, , 16 12 5304 5310, 0743-7463
Kleitz F. Solvyov L. A. Anilkumar G. M. Choi S. H. Ryoo R. 2004Transformation of highly ordered large pore silica mesophases (Fm3m, Im3m and p6mm) in a ternary triblock copolymer-butanol-water system, , 13 1536 1537, 1359-7345
Kim T. W. Kleitz F. Paul B. Ryoo R. 2005MCM-48-like large mesoporous silicas with tailored pore structure: Facile synthesis domain in a ternary triblock copolymer-butanol-water system, , 127 20 7601 7610, 0002-7863